1 COMPUCOM INSTITUTE OF TECHNOLOGY & MANAGEMENT, JAIPUR (DEPARTMENT OF ELECTRONICS & COMMUNICATION) Notes IC TECHNOLOGY (Subject Code: 7EC4) Prepared Class: B. Tech.IV Year, VII Semester
2 SYLLABUS UNIT 2 : DIFFUSION & ION IMPLANTATION- Ficks diffusion Equation in One Dimension, Atomic model, Analytic Solution of Ficks Law, correction to simple theory, Diffusion in SiO2. Ion Implantation and Ion Implantation Systems Oxidation. Growth mechanism and Deal-Grove Model of oxidation, Linear and Parabolic Rate co-efficient, Structure of SiO2, Oxidation techniques and system, Oxide properties Beyond the Syllabus SPUTTERING Learning Objectives To lay the foundation to understand the various growth and fabrication processes in IC Technology
3 UNIT-2 Thermal Oxidation of Silicon The oxide of silicon, or silicon dioxide (SiO 2 ), is one of the most important ingredients in integrated circuits. Thermal SiO 2 is amorphous. It has a density of 2.2 gm/cm 3 and molecular Density of 2.3x10 22 molecules/cm 3. The crystalline SiO 2 is also possible and known as Quartz has a density of 2.65 gm/cm 3. SiO 2 has excellent properties which makes them necessary in every part of the integrated circuits. It is an excellent electrical insulator having energy gap ~ 9 ev with a resistivity greater than ohm-cm and breakdown electric field greater than 10MV/cm. Si technology became popular because of the stable and reproducible Si/SiO 2 interface. Conformal oxide growth on exposed Si surface is easily possible. SiO 2 is a good diffusion mask for common dopants such as. B, P, As, Sb. In addition there exists good etching selectivity between Si and SiO 2. The formation of SiO 2 on a silicon surface is most often accomplished through a process called thermal oxidation. As its name implies, is a technique that uses extremely high temperatures (usually between C) to promote the growth rate of oxide layers whose thicknesses range from 20 to nm. During the process, silicon substrate is exposed to a high purity oxidizing species like oxygen gas (dry oxidation) or water vapour (wet oxidation). The chemical reaction at the silicon surface for dry and wet oxidation is given as Oxidation of silicon is not difficult, since silicon has a natural inclination to form a stable oxide even at room temperature, as long as an oxidizing ambient is present. In both cases the oxidizing species diffuses through the growing oxide and reacts with the silicon surface. These oxidation reactions occur at the Si-SiO 2 interface, i.e., silicon at the interface is consumed as oxidation takes place. As the oxide grows the Si-SiO 2 interface moves into the silicon substrate. As a result, the Si-SiO 2 interface will always be below the original Si wafer surface. The SiO 2 surface, on the other hand, is always above the original Si surface. SiO 2 formation therefore proceeds in two directions relative to the original wafer surface as shown in Fig.3.12.
4 Fig2.1 : The silicon-silicon dioxide interface in thermal oxides The amount of silicon consumed by the formation of silicon dioxide is also fairly predictable from the re ities and molecular weights of Si and SiO2, i.e., the thickness of silicon consumed is 44% of the final thic he oxide formed. Thus, an oxide that is 1000 angstroms thick will consume about 440 angstroms of silicon ubstrate. In another words, 1µm thick Si oxidizes to 2.17 µm thick SiO2. Thermal oxidation is accomplished using an oxidation furnace which provides the heat needed to eleva oxidizing ambient temperature. A furnace typically consists of a temperature controlled heating system, quartz process tubes, arrange for controlled flow of various gases. The heating system usually consi several heating coils that control the temperature around the furnace tubes. The wafers are placed in glassware known as boats. A boat can contain many wafers. The oxidizing agent (oxygen or steam) then the process tube through its source end, subsequently diffusing to the wafers where the oxidation o During dry oxidation, the silicon wafer reacts with the ambient oxygen, forming a layer of silicon dioxide surface. In wet oxidation, the water is heated in the C range and oxygen or nitrogen carrier gases ar for the flow of water vapors to the chamber. Alternatively hydrogen and oxygen gases are introduced torch chamber where they react to form water molecules, which are then made to enter the reactor wher diffuse toward the wafers. The water molecules react with the silicon to produce the oxide and a byproduct, i.e., hydrogen gas. Kinetics of SiO 2 Growth The Linear and Parabolic growth laws were developed by Deal and Grove, and are known as the Linear Parabolic Model. This oxide growth model has been empirically proven to be accurate over a wide range of temperatures ( C), oxide thicknesses (300-20,000 angstroms), and oxidant partial pressures ( atmospheres).
5 Fig.2.2 and 2.3 pictures various diffusions possible and the concentration of species during thermal oxidation and is the basis for Deal and Grove model. Fig. 2.2 : A Model for thermal oxidation of silicon indicating various diffusions possible DEAL GROOVE MODEL OF OXIDATION Fig. 2.3 : A Model for thermal oxidation of silicon indicating the concentration of species The gas-phase flux F 1 is proportional to the difference between the oxidant concentration in the bulk of the gas (C G ) and the oxidant concentration adjacent to the oxide surface (C S ).
6 The Fick's law of solid sate diffusion states that h G is the mass transfer constant (cm/s),d is the diffusion coefficient (cm 2 /s),k S is the surface reaction transfer constant (cm/s), Using and PV = NkT, Henry's law to relate C 0 and C S Where H is the Henry's constant and P S is the partial pressure of oxidant gases at surface If the equilibrium concentration of oxidizing species in oxide is Taking as h, at steady state Solving these two equations for two unknowns
7 To convert F into oxide thickness growth rate Where N 1 is the oxidant molecules cm -3 for dry oxidation and 4.6 at t=0. The oxide thickness grown and B are constants. per unit volume required to form a unit volume of SiO 2. N 1 is 2.3 x x10 22 cm -3 for wet oxidation. Taking boundary conditions as x = x 0 at any point of time t is modeled as where A The time displacement is included to account for the oxide layer (at t = 0) formed by the accelerated growth in the initial phase of oxidation. Fig.2.4 : oxide thickness versus time
8 LINEAR AND PARABOLIC RATE CONSTANTS Typical oxide thickness versus time dependency is shown in Fig For small values of t, the oxide growth equation can be approximated as and thus is known as linear rate constant. For large values of t, the above equation can constant. That is oxide thickness readily seen from: be approximated as and thus B is known as parabolic rate growth slows down with increase in oxide thickness and can be Typical oxide thickness versus time dependency is shown in Fig For small values of t, the oxide growth equation can be approximated as and thus is known as linear rate constant. For large values of t, the above equation can constant. That is oxide thickness readily seen from: be approximated as and thus B is known as parabolic rate growth slows down with increase in oxide thickness and can be Dry oxidation of silicon is typically used to grow a thin, high quality oxide that is used in transistor gates and capacitors. Oxide grown in dry oxygen ambient has excellent insulating properties and is denser, free of defects. Wet oxidation of silicon is typically used to grow thick oxides that are used as diffusion barriers. Silicon dioxide acts as an effective mask against many impurities, allowing dopants into silicon only in regions that are not covered with oxide. The oxide thickness grown on silicon is dependent on the oxidation time and temperature. Wet oxidation method offers faster growth rate compared to dry oxidation. The linear and parabolic rate constants have larger values in wet oxidation case than in case of dry oxidation. This is because equilibrium concentration of oxidizing species in oxide ( ) is approximately three orders of magnitude greater for water than in dry oxygen. Therefore, for growing thick oxide within a realistic time, wet oxidation is a better choice. The linear and parabolic rate constants increase with temperature in both dry and wet oxidation methods. B increases in both casess through the diffusion coefficient (D) increasee due to temperature. The reason for increase in is through k s. OXIDATION TECHNIQUES
9 Dry oxidation of silicon is typically used to grow a thin, high quality oxide that is used in transistor gates and capacitors. Oxide grown in dry oxygen ambient has excellent insulating properties and is denser, free of defects. Wet oxidation of silicon is typically used to grow thick oxides that are used as diffusion barriers. Silicon dioxide acts as an effective mask against many impurities, allowing dopants into silicon only in regions that are not covered with oxide. The oxide thickness grown on silicon is dependent on the oxidation time and temperature. Wet oxidation method offers faster growth rate compared to dry oxidation. The linear and parabolic rate constants have larger values in wet oxidation case than in case of dry oxidation. This is because equilibrium concentration of oxidizing species in oxide ( ) is approximately three orders of magnitude greater for water than in dry oxygen. Therefore, for growing thick oxide within a realistic time, wet oxidation is a better choice. The linear and parabolic rate constants increase with temperature in both dry and wet oxidation methods. B increases in both casess through the diffusion coefficient (D) increasee due to temperature. The reason for increase in is through k s. It can be seen that for small duration, controlled process. the oxidation is a reaction controlled process and longer duration From the Deal and grove model, we have seen that the oxide growth rate is affected by time, temperatu Thickness of oxide is raised by an increase in oxidation time, oxidation temperature, or oxidation pressure. O affect thermal oxidation growth rate for SiO 2 include: the crystallographic orientation of the wafer; the wafer's presence of halogen impurities in the gas phase and the presence of plasma during growth.
10 Figure2.5 Silicon oxide growth The resulting cross section after the wet oxidation is shown in Fig clearly indicating the oxide-silic Fig. 2.6 : The Si-SiO 2 interface changes before and after thermal oxide growth 3.5 Ion-Implantation and Diffusion Diffusion and Ion Implantation are the methods by which impurity is introduced into silicon to change
11 its resistivity. These processes allow the formation of sources and drains of MOSFETs and active regions of bipolar transistors. In diffusion (in a high temperature environment) the dopant atoms are moving from a highly concentrated region to a low concentrated region. The classic approach to creating regions of silicon with different electrical properties was to deposit a dopant material, on the surface, then diffuse or drive it into the surface of the silicon by exposing it to controlled periods of high temperature. As device geometries have become smaller, the side-ways diffusion has become more difficult to deal with, so the industry has converted to the ion implantation process. In implant, the dopant molecules are implanted vertically into the surface of the silicon by a high-energy ion beam. This penetrates the silicon vertically without any appreciable side-ways diffusion. Thus p-type or n- type regions in silicon are created when they are doped with Boron and Phosphorous ions respectively. The following section will deal with diffusion of dopants in a Si lattice. Basics of Diffusion FICKS DIFFUSION EQUATIONS A drop of color in a glass of water spreads from concentrated region to surroundings. This occurs because of the diffusion of color molecules. Similar situation take place when free charge carriers spread in a semiconductor and dopant atoms diffuse in semiconductor at elevated temperature. In this section we use the term diffusion in the later sense. In general, the diffusion is motion of species in solids in the direction of concentration gradient. The chemical process of diffusion is described by the second order differential equation known as Fick's laws. Fick's first law is used in steady state diffusion, i.e., when the concentration within the diffusion volume does not change with respect to time (F in =F out ). Where F is the diffusion flux (in number of dopants cm -2 s -1 ), D is the diffusion coefficient or diffusivity (in cm 2 s -1 ), n is the concentration of dopants (in cm -3 ), x is the position (cm). The diffusion coefficient (D) determines rate with which element moves in a given solid by diffusion. D depends strongly on temperaturee and varies between elements by orders of magnitude. For example in the case of diffusion in silicon diffusion coefficient for gold (Au), is in the range of 10-3 cm 2 /sec (fast diffusant) while for Antimony (Sb) is in the range of cm 2 /sec. Since D is a function of temperature, the flux (F) is also a function of temperature. Negative sign indicates that the flow is down the concentration gradient. Fick's second law is used in non-steady or continually changing state diffusion, i.e., when the concentration within the diffusion volume changes with respect to time. Becausee diffusion in solids is slow, diffusion is almost always transient.
12 This can be derived from the First Fick's law and the mass balance assuming the diffusion coefficient D to be a constant. This equation state that the dopant will redistribute until it is spread uniformly throughout the material. The time scale of this redistribution is given by the coefficient of diffusion The tendency toward diffusion is very strong even at room temperature because of the high molecular velocities associated with the thermal energy of the particles. The diffusion coefficient is temperature dependent, and is can be described by the Arrhenius expression: D = D 0 exp(- E a /RT) k is Boltzmann's constant. D 0 (is the maximum diffusion coefficient (at infinite temperature) and E a (the energy of activation) is constants describing the diffusion. All kinds of diffusion require a certain minimum energy to occur and it can be called the activation energy. The higher the activation energy, the harder it is for diffusion to occur.. Typically one use higher doping concentrations and lower thermal budgets for semiconductor fabrication. It was observed that Fick's laws are not accurate enough for the explaining the anomalous diffusion behavior. Therefore it is necessary to focus on atomistic level to get insight on the interaction of dopants with lattice atoms. It is established that diffusion of impurities can only occur within the crystal lattice due to the presence of point-defects. Diffusion by point defects Diffusion occurs in silicon primarily at native point-defects and impurity-related point defects. Typically native defects such as point defects, line defects and surface defects are present in an otherwise perfect crystal lattice. At room temperature point defect concentration is low that practically no diffusion occurs. However, an increase of point defects will cause an increase in the diffusion. The concentration of point defects will increase for example if the crystal is heated or irradiated by ion. Both situations are likely to occur during the fabrication of devices. Impurity related defects arise from the introduction of group- III elements or group-v elements into the silicon lattice. Normally dopants will occupy a lattice site, and the dopant is said to be substitutional. When the dopant i the substitutional position it is not likely that it will move around. However, when it gets in contact wit point defect, it will be mobile. A point defect in silicon, can be a Si self-interstitial (a silicon atom wh does not occupy a lattice site), or a vacancy (a lattice site which does not contain a silicon atom). illustrated in Fig. 3.37, t here are mainly two possible atomic diffusion mechanisms known as interstitial vacancy diffusion. The diffusion mechanisms through grain boundaries and surface are also possible. T highest activation energy is for volume diffusion though interstitial and vacancy sites. The grain bound diffusion requires less energy and surface diffusion requires the least.
13 Fig. 2.7 : Diffusion mechanisms within crystal targets Diffusion through interstitial spaces: Impurities which have small ionic radii can travel directly from one interstitial site to another one (see Fig.3.37). Especially Group-I and Group-VIII elements are diffusing mainly interstitially and are therefore fast diffusers. Vacancy Diffusion: Vacancies are holes in the matrix and they are always moving. An impurity can move into the vacancy and diffuse through the material. A substitutional dopant can exchange its position with the neighboring vacancy. Similarly when a dopant at a substitutional site is kicked out by a silicon interstitial atom, the dopant occupies the interstitial position while the original self-interstitial has disappeared by occupying the regular lattice site. Thus dopants can diffuse within a crystal lattice using point-defects as diffusion vehicle either by the vacancy mechanism or the interstitiall mechanism or a combination of both. The dopants are selected based on their properties such as solubility in silicon, dissolution into lattice sites and ionization. The most common p-type dopant boron diffuses mainly via interstitials, where the n-type dopant phosphorus shows at intrinsic concentrations interstitial dominated diffusion and for high concentrations a dual mechanism with a strong vacancy component. Arsenic is also diffusing via interstitials and vacancies, but the interstitial diffusion is at least limited due to the relatively large ionic radii. Large dopants like Antimony will find no stable position between lattice sites, so they can only diffuse via vacancies The transport of dopants within the lattice is not only controlled by the diffusion mechanism, there are also recombination processes between dopants and point-defects occurring, which can disturb or even prevent dopants from diffusion. These recombinations are always possible when dopant-defect pairs are approaching lattice defects of the opposite type. If the dopant concentration level is significantly below the intrinsic carrier concentration, the diffusivities of the dopants show no dependence on the doping level. In the subsequent section we will focus on two practical circumstances in which the diffusion can be carried out. Diffusion from an unlimited source (Constant source diffusion) occurs when a wafer is exposed to an infinite amount of dopants during the diffusion period. In the case of diffusion from a limited source, a finite quantity of the dopants is first placed on the wafer and diffusion proceeds from this limited source and it is assumed that all the dopants are consumed.
14 Diffusion from an unlimited source The surface concentration will be fixed at the solid solubility, and the distribution will be in the form of a complimenta where : N = concentration (cm -3 ) N 0 = solid solubility limit for dopant (cm -3 ) x = position inside silicon relative to the surface D = diffusion coefficient for dopant (cm 2 /s) t = time (seconds) If one sketch of this concentration profile for various diffusion times, one can observe that the surface concent where as the diffusion depth increases with time. Please note that the Dose beyond x=0 continues to increase w Note that the dose is given by The error function values for typical values are given in the Table 9.
15 Table 2.1 : Typical error function values Z erf(z) Z erf(z) Diffusion from a limited source Fig. 2.8: Double sided iffusion from a delta source at origin The solution that satisfies Fick's second law when a fixed dose Q is introduced as a delta function at the origin is given by
16 Please note the following important consequences: 1. Dose Q remains constant before and after diffusion 2. Peak concentration decreases as 3. Diffusion distance from origin increases as This equation can be slightly modifiedd to model a practical situation where all the dopants from the constan are consumed entirely to one side. Fig. 2.9 : Single side d iffusion from a delta source at origin The solution is given by Also note that the infinite source diffusion case discussed previously can be thought infinite source of dopant made up of small slices each diffusing as a Gaussian. Error function solution is made up of a sum of Gaussian delta function solutions.
17 Fig : Diffusion profiles in constant source and limited source cases Diffusion Systems ANALYTIC SOLUTION TO FICKS DIFFUSION EQUATIONS The diffusion process is carried out in systems called diffusion furnaces which may be either sealed or open tube type. The silicon wafer and the dopants are placed into the quartz tube before sealing and subsequently after the high temperature process; the tube is broken to remove the diffused wafers. Thus the sealed tubes are for one time use and can be maintained contamination free. The open tube method is preferred because multiple diffusion runs can be carried out. Separate tubes for each type of dopants are maintained because tubes are contaminated with the respective impurity. The insertion of wafers and solid dopant sources are done from one end of the tube and the other end is used for the flow of gases or impurities in vapour form. The diffusion furnaces are usually operated at temperatures 600C C and constant temperature zones are maintained with a ± 0.5 C tolerance. Three main sources of dopants such as gaseous, liquid and solids source of dopant atoms are used in semiconductor doping processes. The gaseous sources are most widely used since they are reliable and convenient. The typical examples are BF 3 (diborane), PH 3 (phosphine) and AsH 3. Source gas reacts with oxygen at the wafer surface to form a dopant oxide, the dopant then diffuses from the oxide into silicon resulting in a uniform dopant concentration across the surface. Liquid sources are available in two forms: Bubblers and spin on dopants. Bubblers convert the liquid to vapour, which then reacts with oxygen to form dopant oxides on the wafers. The spins on dopants are solutions which on drying form doped SiO 2 layers. The typical examples of liquid sources are POCl 3 and BBr 3 (boron tribromide).
18 Solid sources are available in two forms; such as tablet/granular and disc/wafer form. BN discs are most commonly used oxidized at C to serve as the boron diffusion source. Dopants are introduced into the silicon substrate using a two step, high temperature process. The first diffusion (predeposition) introduces dopants into the wafer. The second diffusion (drive) redistributes the dopants and allows the dopants to diffuse into the wafer more deeply (up to ~3 micrometers). The goal of the dopant predeposition diffusion is to move dopant atoms from a source to the wafer, and later allow the dopants to diffuse into the wafer. In order for the dopants to move into the silicon, they must be given energy, usually in the form of heat. In order for the diffusion to occur in a reasonable time, the temperature must be very high (900ºC <T<1200º). At this temperature the dopant (in the form of an oxide) reacts with the exposed silicon surface to form a highly doped glass. It is from this glass that the dopants can then diffuse into the wafer. Arsenic has a low misfit factor ( ) and can be incorporated to a high concentration without causing strain the lattice. Arsenic's low diffusivity (about one-tenth of boron or phosphorous) and its abrupt doping profile makes it ideally suited for shallow diffused structures where more precise control of junction depth is needed. Phosphorus also has a high solid solubility and active carrier concentration close to arsenic. Its misfit factor also is small ( ). these characteristics makes its very useful for the fabrication of n+ regions in MOS and bipolar circuits. Phosphorus, in the form of P 2 O 5, diffuses from the source to the wafer. When it reaches the silicon, it will undergo the following chemical reaction: The phosphosilicate glass (PSG) is in contact with the silicon surface. A concentration gradient is formed, and since this process occurs at high temperature, diffusion will occur. The surface concentration will be fixed at the solid solubility, and the distribution will be in the form of a complimentary error function :
19 where : N = concentration (cm -3 ) N s1 = solid solubility limit for dopant (cm x = position inside silicon relative to the s D = diffusion coefficient for dopant (cm 2 / t = time (seconds) where : N = concentration (cm -3 ) N s1 = solid solubility limit for dopant (cm -3 ) x = position inside silicon relative to the surf D = diffusion coefficient for dopant (cm 2 /s) t = time (seconds)
20 where : N = concentration (cm -3 ) N s1 = solid solubility limit for dopant (cm x = position inside silicon relative to the s D = diffusion coefficient for dopant (cm 2 / t = time (seconds) Boron Diffusion from a solid source to form a BJT base: a case study Boron is the most commonly used p-type dopant for silicon, principally because it is the only column III element that can be masked by SiO 2. The first step, called the predeposition, is an open tube diffusion process that involves the gaseous transfer of a compound containing the dopant to the Si wafer. The gas may be supplied in several different ways, but in almost all cases the final chemical reaction when it reaches the silicon is: Boron, in the form of B 2 O 3, diffusess from the source to the wafer. The surface concentration during such constant source diffusion is usually limited by the solid solubility of the dopant in silicon. The boron predeposition transfers boron from a solid source to the wafer. The borosilicate glass (BSG) is in contact with the silicon surface. A concentration gradient is formed, and since this process occurs at high temperature, diffusion will occur. If the boron source used is a solid source of boron nitride wafers, Si wafers are stacked next to oxidized wafers as shown. At the pre-deposition temperature, concentration gradient induced diffusion is established between the source wafers and the silicon wafers. This concentration gradient is a function of the distance between the source and silicon, the temperature of the pre-deposition, and the composition of the gas ambient (oxidizing or non-oxidizing, presence of H 2 O, etc.). Ideally, however, it is not a function of gas flow rate, which is low enough so that the gas between source and wafer is essentially stagnant. The concentration gradient results in the transfer of B 2 O 3 to the silicon surface, and so produces a very thin, very highly doped region at the silicon wafer surface. The final level of doping and resulting sheet resistance is determined by time and the size of the concentration gradient. Note, however, that the pre-deposition temperature is so low that very little boron diffusion into the silicon actually takes place.
21 After the predeposition diffusion the dopants are situated close to the surface of the wafer. However, they must diffuse even farther to lower the overall concentration in order for some of the devices to work properly. In addition, oxygen and water vapor are introduced during the drive diffusion to grow a new oxide over the areas which were exposed to bare silicon during the photolithography process. This new oxide can be patterned again so that other selective diffusion processes can be performed to create other types of devices. The second stage of the diffusion process, called the drive-in, has as its objectivee the redistribution of the dopant deeper into the silicon, and is referred to as a constant source diffusion. For this process we first remove our silicon wafer from the pre-deposition furnace and strip off the SiO 2 - B 2 O 3 glass using HF. The HF actually attacks the SiO 2, not the B 2 O 3, so care must be used in the pre-deposition step to prevent the deposition of excessive amounts of B 2 O 3. This is done mainly by assuring no H 2 O is present in the furnace, which would greatly increase the rate of transfer of B 2 O 3 to the silicon. Also note the thin SiB x phase on the wafer is hydrophilic, so the wafer will not de-wet after etching. The actual drive-in is performed at very high temperatures (~1100 C). The drive-in is usually initiated in an oxidizing environment; the initial growth of SiO 2 prevents the out-diffusion of the boron during the rest of the process. The boron concentration near the surface after predeposition is too high and the junction depth is too shallow to act as a good base. After the BSG is removed from the surface of the wafer, a 'sourceless' diffusion (drive) will lower the surface concentration and simultaneously drive the dopant deeper into the wafer. The distribution can be approximated as a Gaussian profile:
22 N = concentration (cm -3 ) N 0 = surface concentration (cm -3 ) x = position inside silicon relative to the surface D = diffusion coefficient for dopant (cm 2 /s) t = time (seconds) and N 0 = surface concentration after the drive (cm -3 ) N 01 = surface concentration after the drive (cm -3 ) D 1 = diffusion coefficient f of dopant during the predep (cm 2 /s) t 1 = time of the predep (seconds) D 2 = diffusion coefficient f of dopant during the drive (cm 2 /s) t 2 = time of the drive (seconds) In addition to redistribution of the dopant, another oxide layer is grown which may act as a mask for the further process. If a dopant is diffused at temperature T 1 for time t 1 and then is diffused at temperature T 2 for time t 2 etc. the total effective Dt is given by the sum of all the individual Dt products. Some of the Dt steps may be negligible in a process. The Gaussian solution only holds if the Dt used to introduce the dopant is small compared with the final Dt for the drive-in i.e. if an initial delta function approximation is reasonable. Example 5 : In a bipolar transistor, if the emitter profile is formed by a predeposition and the base profile by an implant + drive-in, then the junction for the emitter-base occurs when
23 And the emitter-base occurs when Example 6 : Boron Diffusion from a solid source to form well: a case study We can now consider how to design a boron diffusion process (say for the well or tub of a CMOS process) such that
24 The average conductivity of the layer is Fig : Resistivity of bulk and surface charges The resistivity of a cube is given by cm The sheet resistance of a shallow junction is For a non-uniformly doped layer Sheet resistance can be experimentally measured by a four point probe technique. This equation has been numerically integrated by Irwin for different analytical profiles (for example P type Gaussian profiles). Such plots with surface concentration (cm -3 ) verses effective conductivity ( - cm) -1 are called Irvin's curves
25 From the Irvin curve we obtain thatt Assuming a Gaussian profile after the drive in Ion Implantation Ion implantation is the introduction of atoms into a solid substrate by bombardment with ions in the kev to MeV energy range. It was early recognized that this technique provides the possibility of introducing a wide selection of atomic species and also external control of both the number of atoms per cm 2 introduced into the semiconductor and the depth distribution of the implanted species. This is in contrast to diffusion processes where temperature governs the surface concentration and time and temperature determine the depth distribution. The initial impact of ion implantationn in silicon technology was in charge control. This in combination with the fact that simple masking techniques can be used to define the geometrical area of the implanted region led to extensive to MOS technology. Presently implantation is the most common method of introducing dopant atoms for the fabrication of Si devices. Advantages This process provides excellent dose control. Typical to cm -2. It has been possible to control the number of dopant atoms per cm 2 to about 1% over the surface of a wafer, and to control the number within 3% from wafer to wafer. The ion implantation results in less lateral diffusion i.e. diffusion of dopant atoms in the direction parallel to the surface of semiconductor compared to the vertical diffusion where diffusing species are moving in a direction normal to the wafer surface. The dopant elemental selection can be easily carried out by mass separation from impure sources and this helps in preventing contamination. The room temperature process allows resist to be used and it allows doping anytime during process. Modeling is very accurate Complex doping profiles can be made using multiple energy implants Highly abrupt junctions can be made Highly automatic parameters
26 Limitations Because ion implantation causes damage to the crystal structure of the target which is often unwanted, ion implantation processing is often followed by a thermal annealing. This can be referred to as damage recovery. As the energetic ions are introduced in the Si lattice, many Si atoms are knocked off their lattice positions resulting in large numbers of Si interstitial atoms and vacant lattice sites (Frenkel pairs). Since the as-implanted dopants are usually electrically non-active and the lattice damage deteriorates the device performance, it is necessary to have the annealing of the implanted sample at temperatures high enough to permit the dopant atoms to incorporate into substitutional sites and thus become electrically active, and for the defects to annihilate and thus repair the damage. The diffusion of impurities in implanted Si during thermal anneal is complicated as a result of the presence of implantation damage. As an example, the diffusivity of B in implanted crystalline Si is anomalously high compared to equilibrium values. This phenomenon has important consequences for Si processing, since it causes the dopant profile to spread significantly compared to the as-implanted profile during the subsequent annealing steps required for dopant activation. The presence of damage also causes dopant clustering and thus prevents complete electrical activation. The down-scaling of Si CMOS devices requires simultaneously the formation of ultra shallow junctions for the source and drain extensions and a low sheet resistance (high carrier concentration). Conventionally, there is a compromise involved in maximizing dopant electrical activation while minimizing dopant diffusion. The amount of crystallographic damage can be enough to completely amorphize the surface of the target: it can become an amorphous solid. However in some cases, complete amorphization of a target is prefera to a highly defective crystal: An amorphized film can be regrown at a lower temperature than required anneal a highly damaged crys Implantors are very expensive machines, requiring heavy maintainace and upkeep. The Safety haz precautions are also stringent because of the radiation, high energy beams and high voltag Sputtering : Some of the collision events result in atoms being ejected from the surface, and thus implantation will slowly etch away a surface. The effect is only appreciable for very large doses. Fig : Basic illustration of channelling Ion channeling : Since the semiconductor substrates have crystal structure, particular crystallographic directions offer much lower stopping than other directions. The result is that the range of an ion can be
27 much longer if the ion travels exactly along a particular direction, for example the <110> direction in silicon and other diamond cubic materials as shown in Fig This effect is called ion channelling, and, like all the channelling effects, is highly nonlinear, with small variations from perfect orientation resulting in extreme differences in implantation depth. For this reason, most implantation is carried out a few degrees off-axis, where tiny alignment errors will have more predictable effects. Ion channelling can be used directly in Rutherford backscattering and related techniques as an analytical method to determine the amount and depth profile of damage in crystalline thin film materials. A comparison of Solid/Gas Phase Diffusion verses Ion Implantation and Annealing is provided in Table 10. Table 2.2 Diffusion verses Ion Implantation Diffusion Ion Implantation Room temperature mask Precise dose control No damage created by doping Wide range of doses Batch fabrication Accurate depth control Usually limited to solid solubility Implant damage enhances diffusion Low surface concentration hard to ac without a long drive-in Dislocations caused by damage may cause junction leakage Low dose predeposition very difficu Implant channeling may affect profile RANGE THEORY Impurity Profiles : Range and Depth Distribution Lowthroughput Junction depth limited to 1 micron There are two basic mechanisms by which energetic ions are stopped in a substrate. Ions interact with electrons and nuclei of substrate atoms and lose energy during these collisions. The range (R) is the total distance traveled by an ion before resting. Please note that the path is not a straight line. The Nuclear collisions transfer energy away from ion and the coulombic interaction with electrons transfer energy to electrons.
28 If S n (E) is energy loss per unit length due to nuclear stopping and S e (E) is energy loss per unit length due to electronic stopping, the total rate of energy loss ( ) is the sum of the two losses: Fig.2.13 : Ion Nuclei interactions If one consider ions as balls with momentum p=mv the nuclear stopping is provided by velocity interaction. If the rate of energy loss is plotted as a function of ion energy, it can be seen that the loss increases linearly at low energy because the ion velocity is smaller, the loss reaches maximum and decreases at higher energy becausee the higher velocity makes ion move too quickly to interact. S n (E) increases with ion mass (p=mv) and if ions are light (e.g. Boron), its energy loss/unit length ( much ) is lower. S e (E) is energy loss per unit length due to electronic stopping. Drag force caused by charged ion in "sea" of electrons (non-local electronic stopping).
29 Fig : Ion electron interactions Collisions with electrons around atoms transfers momentum and results in local electronic stopping. Fig : Electron Electron interactions This is similar to stopping a projectile in viscous medium:
30 k depends on ion and target mass and atomic number. The lighter ion, boron, has larger. The crossover point between electronic and nuclear stopping is an important parameter. The critical energy E c when the nuclear and electronic stoppings are equal is That is for B, S e (E) dominates down to 10 kev and for As, nuclear stopping dominates up to 700 kev. The range (R) is: A more significant parameter of interest is the projected range (R P ) and it is the distance travelled normal to the surface as shown in Fig Fig : Range (R) and projected range (R P ) in ion implantation
31 Fig 2.17 guassian curve The peak concentration occurs where x= R p where Q 0 is the ion dose (cm -2 ), N p is the maximum (desired) concentration, R p is the range or desired depth, and R p is the straggle or standard deviation. The projected range and straggle can be approximated from range: Where M 1 is the ion mass and M 2 is the substrate mass. A wide variety of masking materials can be used during the implantation and the thickness of the mask can be estimated using the above equations once the range (or stopping) parameters of the mask
32 material is known. The important goals of damage annealing are: Remove primary damage created by the implant and activate the dopants. Restore silicon lattice to its perfect crystalline state. Restore the electron and hole mobility. Do this without appreciable dopant redistribution. Fig : B, P, As and Sb implanted concentration profile in Si
33 Fig. 2.19: Gaussian profile in the case of implantation followed by thermal anneal, using the expression,the peak concentration and junction depth can be calculated; N p = 6.6x10 18 cm -3 and junction depth (x j) = m Ion Implantation systems Ion implanters are usually specified in terms of two key parameters; the ion energy which determines the penetration depth and the ion current which decides the dose. The basic building blocks of an implanter are ion sources, ion extractors, accelerators to high energies and beam manipulators as shown in Fig Ions are produced by passing the gas vapour through a discharge chamber. The electrons are accelerated towards an anode which is typically at 100V. A magnetic field is provided to force electrons into a spiral trajectory and this will enhance the ionisation efficiency. The positive ions are moved out of the discharge chamber by means of another anode biased at kv. The pressure in the remaining part of the system is kept below 10-6 Torr to minimize the ion scattering. The output of an ion discharge chamber consists of many species in addition to the contamination produced by sputtering from its walls. Thus a mass separator is required to make source pure. The mass separation is based on the dynamics of charged particles, of mass (m) and velocity (v), moving at right angles to a uniform magnetic field (a flux density of B). These particles will experience a force (F) such that. This force tends ions to move in a circular path of radius r, and experience a
34 centrifugal force. These forces are equal and opposite. The velocity of ions is related to the accelerating potential (V) by. Combining these equations, the radius of the Fig : Schematic diagram of a basic implantation system ion path is given as For a given extraction voltage and magnetic flux density, the r is proportional to square root of mass and thus ions of any particular masss can be selected by appropriately placing an exit slit. The collimators filter a stream of rays so that only those travelling parallel to a specified direction are allowed through. They help to shape the beam of radiation emerging from the machine and can limit the maximum field size of a beam. The surviving ions move into the accelerator tube where the ion beams gets energised under the very high acceleration potential. The output of the tube is usually maintained at ground potential for safety reasons. In order to implant in the x and y directions the wafer surface, electrostatic and mechanical beam scanning techniques are used. The electrostatic scanning in both x and y directions is the simplest, and has advantage of very high scanning speed. However, when the beam voltages are 50 kev or higher, beam expansion (blow up) takes place and so mechanical scanning is usually used. In the mechanical scanning system the beam is stationary and the substrate wafer is moved.
Chapter 4 1 CHAPTER 4: Oxidation Oxidation of silicon is an important process in VLSI. The typical roles of SiO 2 are: 1. mask against implant or diffusion of dopant into silicon 2. surface passivation
HOMEWORK 4 and 5 March 15, 2009 Homework is due on Monday March 30, 2009 in Class. Chapter 7 Answer the following questions from the Course Textbook: 7.2, 7.3, 7.4, 7.5, 7.6*, 7.7, 7.9*, 7.10*, 7.16, 7.17*,
Section 4: Thermal Oxidation Jaeger Chapter 3 Properties of O Thermal O is amorphous. Weight Density =.0 gm/cm 3 Molecular Density =.3E molecules/cm 3 O Crystalline O [Quartz] =.65 gm/cm 3 (1) Excellent
Microelettronica Planar Technology for Silicon Integrated Circuits Fabrication 26/02/2017 A. Neviani - Microelettronica Introduction Simplified crosssection of an nmosfet and a pmosfet Simplified crosssection
ECE 440 Lecture 27 : Equilibrium P-N Junctions I Class Outline: Fabrication of p-n junctions Contact Potential Things you should know when you leave Key Questions What are the necessary steps to fabricate
1 CHAPTER 8: Diffusion Diffusion and ion implantation are the two key processes to introduce a controlled amount of dopants into semiconductors and to alter the conductivity type. Figure 8.1 compares these
Section 4: Thermal Oxidation Jaeger Chapter 3 Properties of O Thermal O is amorphous. Weight Density =.0 gm/cm 3 Molecular Density =.3E molecules/cm 3 O Crystalline O [Quartz] =.65 gm/cm 3 (1) Excellent
Chapter 5 UEEP613 Microelectronic Fabrication Diffusion Prepared by Dr. Lim Soo King 4 Jun 01 Chapter 5 Diffusion...131 5.0 Introduction... 131 5.1 Model of Diffusion in Solid... 133 5. Fick s Diffusion
Changing the Dopant Concentration Diffusion Doping Ion Implantation Step 11 The photoresist is removed with solvent leaving a ridge of polysilicon (the transistor's gate), which rises above the silicon
Ion implantation Contents 1. Introduction 2. Ion range 3. implantation profiles 4. ion channeling 5. ion implantation-induced damage 6. annealing behavior of the damage 7. process consideration 8. comparison
Technische Universität Graz Institute of Solid State Physics Doping and Oxidation Franssila: Chapters 13,14, 15 Peter Hadley Technische Universität Graz Institute of Solid State Physics Doping Add donors
ELEC 3908, Physical Electronics, Lecture 4 Basic Integrated Circuit Processing Lecture Outline Details of the physical structure of devices will be very important in developing models for electrical behavior
Processing of Semiconducting Materials Prof. Pallab Banerjee Department of Material Science Indian Institute of Technology, Kharagpur Lecture - 35 Oxidation I (Refer Slide Time: 00:24) Today s topic of
Ion Implantation Most modern devices doped using ion implanters Ionize gas sources (single +, 2+ or 3+ ionization) Accelerate dopant ions to very high voltages (10-600 KeV) Use analyzer to selection charge/mass
SILICON OXIDATION Silicon Oxidation Many different kinds of thin films are used to fabricate discrete devices and integrated circuits. Including: Thermal oxides Dielectric layers Polycrystalline silicon
THERMAL OXIDATION - Chapter 6 Basic Concepts SiO 2 and the Si/SiO 2 interface are the principal reasons for silicon s dominance in the IC industry. Oxide Thickness µm 0. µm 0 nm nm Thermally Grown Oxides
Oxide Growth 1. Introduction Development of high-quality silicon dioxide (SiO2) has helped to establish the dominance of silicon in the production of commercial integrated circuits. Among all the various
Chapter 4 UEEP2613 Microelectronic Fabrication Oxidation Prepared by Dr. Lim Soo King 24 Jun 2012 Chapter 4...113 Oxidation...113 4.0 Introduction... 113 4.1 Chemistry of Silicon Dioxide Formation... 115
Semiconductor Manufacturing Technology Michael Quirk & Julian Serda October 2001 by Prentice Hall Chapter 17 Doping Processes Common Dopants Used in Semiconductor Manufacturing Acceptor Dopant Group IIIA
2014 Ajay Kumar Gautam [VLSI TECHNOLOGY] VLSI Technology for 3RD Year ECE/EEE Uttarakhand Technical University Page1 Syllabus UNIT 1 Introduction to VLSI Technology: Classification of ICs, Scale of integration,
EE 22 FALL 999-00 THERMAL OXIDATION - Chapter 6 Basic Concepts SiO 2 and the Si/SiO 2 interface are the principal reasons for silicon s dominance in the IC industry. SiO 2 : Easily selectively etched using
Microstructure of Electronic Materials Amorphous materials Single-Crystal Material 1 The Si Atom The Si Crystal diamond structure High-performance semiconductor devices require defect-free crystals 2 Crystallographic
EECS130 Integrated Circuit Devices Professor Ali Javey 9/13/2007 Fabrication Technology Lecture 1 Silicon Device Fabrication Technology Over 10 15 transistors (or 100,000 for every person in the world)
Problem 1 Lab Questions ( 20 points total) (a) (3 points ) In our EE143 lab, we use Phosphorus for the source and drain diffusion. However, most advanced processes use Arsenic. What is the advantage of
Chapter 3 CMOS processing technology (How to make a CMOS?) Si + impurity acceptors(p-type) donors (n-type) p-type + n-type => pn junction (I-V) 3.1.1 (Wafer) Wafer = A disk of silicon (0.25 mm - 1 mm thick),
Ch. 5: p-n Junction Most semiconductor devices contain at least one junction between p-type and n-type material. These p-n junctions are fundamental to the performance of functions such as rectification,
Semiconductor Technology from A to Z Oxidation www.halbleiter.org Contents Contents List of Figures List of Tables II III 1 Oxidation 1 1.1 Overview..................................... 1 1.1.1 Application...............................
Low Defect Boron Diffusion Systems The purpose of the hydrogen injection process is to increase die yield per wafer. This is accomplished because the effects associated with the hydrogen injection process.
Contents: VI Sem ECE 06EC63: Analog and Mixed Mode VLSI Design PROCESS FLOW AN INSIGHT INTO CMOS FABRICATION PROCESS 1. Introduction 2. CMOS Fabrication 3. Simplified View of Fabrication Process 3.1 Alternative
Kinetics of Silicon Oxidation in a Rapid Thermal Processor Asad M. Haider, Ph.D. Texas Instruments Dallas, Texas USA Presentation at the National Center of Physics International Spring Week 2010 Islamabad
MICROCHIP MANUFACTURING by S. Wolf Chapter 13: THERMAL- OXIDATION of SILICON 2004 by LATTICE PRESS Chapter 13: THERMAL-OXIDATION of SILICON n CHAPTER CONTENTS Applications of Thermal Silicon-Dioxide Physical
Chapter 3 Silicon Device Fabrication Technology Over 10 15 transistors (or 100,000 for every person in the world) are manufactured every year. VLSI (Very Large Scale Integration) ULSI (Ultra Large Scale
Lecture 4 Oxidation (applies to Si and SiC only) Reading: Chapter 4 Introduction discussion: Oxidation: Si (and SiC) Only The ability to grow a high quality thermal oxide has propelled Si into the forefront
VLSI Technology Dr. Nandita Dasgupta Department of Electrical Engineering Indian Institute of Technology, Madras Lecture - 33 Problems in LOCOS + Trench Isolation and Selective Epitaxy So, we are discussing
Ion Implantation Most modern devices doped using ion implanters Implant dopants by accelerating individual atoms (ions) Ionize gas sources (single +, 2+ or 3+ ionization) Use analyzer to selection charge/mass
SRI VENKATESWARA COLLEGE OF ENGINEERING AND TECHNOLOGY TIRUPACHUR DEPARTMENT OFELECTRICAL AND ELECTRONICS ENGINEERING EE6303 LINEAR INTEGRATED CIRCUITS AND APPLICATIONS 1. Define an Integrated circuit.
AND FABRICATION ENGINEERING ATTHE MICRO- NANOSCALE Fourth Edition STEPHEN A. CAMPBELL University of Minnesota New York Oxford OXFORD UNIVERSITY PRESS CONTENTS Preface xiii prrt i OVERVIEW AND MATERIALS
EE 330 Lecture 9 IC Fabrication Technology Part 2 Quiz 8 A 2m silicon crystal is cut into wafers using a wire saw. If the wire diameter is 220um and the wafer thickness is 350um, how many wafers will this
ELEC 7364 Lecture Notes Summer 2008 Si Oxidation by STELLA W. PANG from The University of Michigan, Ann Arbor, MI, USA Visiting Professor at The University of Hong Kong The University of Michigan Visiting
Suggested Reading EE40 Lec 22 IC Fabrication Technology Prof. Nathan Cheung 11/19/2009 300mm Fab Tour http://www-03.ibm.com/technology/manufacturing/technology_tour_300mm_foundry.html Overview of IC Technology
Metallization deposition and etching Material mainly taken from Campbell, UCCS Application Metallization is back-end processing Metals used are aluminum and copper Mainly involves deposition and etching,
Structural changes of polycrystalline silicon layers during high temperature annealing D. Lysáček, L. Válek ON SEMICONDUCTOR CZECH REPUBLIC, Rožnov p. R., firstname.lastname@example.org Abstract The structure
Fairchild Semiconductor Application Note June 1983 Revised March 2003 High-Speed CMOS (MM74HC) Processing The MM74HC logic family achieves its high speed by utilizing microcmos Technology. This is a 3.5
Chapter 2 Crystal Growth and Wafer Preparation Professor Paul K. Chu Advantages of Si over Ge Si has a larger bandgap (1.1 ev for Si versus 0.66 ev for Ge) Si devices can operate at a higher temperature
VLSI Technology Dr. Nandita Dasgupta Department of Electrical Engineering Indian Institute of Technology, Madras Lecture - 32 IC BJT - From junction isolation to LOCOS So, by now, we have completed all
Chapter 5 PROCESSING OF DEVICES A discussion of crystal growth, lithography, etching, doping, and device structures is presented in the following overview gures. SEMICONDUCTOR DEVICE PROCESSING: AN OVERVIEW
Increased Yield Using PDS Products Grade BN-975 with Hydrogen Injection Technical Bulletin The purpose of the hydrogen injection process is to increase die yield per wafer. This is accomplished because
Silicon Manufacturing Group Members Young Soon Song Nghia Nguyen Kei Wong Eyad Fanous Hanna Kim Steven Hsu th Fundamental Processing Steps 1.Silicon Manufacturing a) Czochralski method. b) Wafer Manufacturing
PHYSICAL ELECTRONICS(ECE3540) Brook Abegaz, Tennessee Technological University, Fall 2013 1 Chapter 1 The Crystal Structure of Solids Physical Electronics: Includes aspects of the physics of electron movement
3.155J / 6.152J Micro/Nano Processing Technology TAKE-HOME QUIZ FALL TERM 2005 1) This is an open book, take-home quiz. You are not to consult with other class members or anyone else. You may discuss the
Tool Identifier Boron, Phosphorous diffusion furnaces Document version 1.1 September 2012 Documented by Karthick Murukesan SAMPLE PREQUIREMENT: Sample should be either RCA cleaned or Piranha cleaned before
Transistors on a Chip Lecture #18 Fabrication OUTLINE IC Fabrication Technology Introduction the task at hand Doping Oxidation Thin-film deposition Lithography Etch Lithography trends Plasma processing
Silicon Epitaxial CVD Want to create very sharp PN boundary grow one type layer on other in single crystal form High dopant layers on low dopant substrate Creates latch up protection for CMOS Buried Epi
3. Photolithography, patterning and doping techniques KNU Seminar Course 2015 Robert Mroczyński Critical technology processes Photolithography The aim of this process is to transfer (in the most accurate
EE 330 Lecture 9 IC Fabrication Technology Part II -Oxidation -Epitaxy -Polysilicon -Planarization -Resistance and Capacitance in Interconnects Review from Last Time IC Fabrication Technology Crystal Preparation
Graduate Student Presentations Dang, Huong Chip packaging March 27 Call, Nathan Thin film transistors/ liquid crystal displays April 4 Feldman, Ari Optical computing April 11 Guerassio, Ian Self-assembly
Physics and Material Science of Semiconductor Nanostructures PHYS 570P Prof. Oana Malis Email: email@example.com Today Bulk semiconductor growth Single crystal techniques Nanostructure fabrication Epitaxial
Thermal Evaporation Theory 1. Introduction Procedures for depositing films are a very important set of processes since all of the layers above the surface of the wafer must be deposited. We can classify
ME 141B: The MEMS Class Introduction to MEMS and MEMS Design Sumita Pennathur UCSB Outline today Introduction to thin films Oxidation Deal-grove model CVD Epitaxy Electrodeposition 10/6/10 2/45 Creating
CHAPTER - 4 CMOS PROCESSING TECHNOLOGY Samir kamal Spring 2018 4.1 CHAPTER OBJECTIVES 1. Introduce the CMOS designer to the technology that is responsible for the semiconductor devices that might be designed
Thin Films: Sputtering Systems (Jaeger Ch 6 & Ruska Ch 7,) Can deposit any material on any substrate (in principal) Start with pumping down to high vacuum ~10-7 torr Removes residual gases eg oxygen from
INSTRUCTIONS Read all of the instructions and all of the questions before beginning the exam. There are 5 problems on this Final Exam, totaling 143 points. The tentative credit for each part is given to
Silicon Epitaxial CVD Want to create very sharp PN boundary grow one type layer on other in single crystal form High dopant layers on low dopant substrate Creates latch up protection for CMOS Buried Epi
4 Silicon Temperature Sensors 4.1 Introduction The KTY temperature sensor developed by Infineon Technologies is based on the principle of the Spreading Resistance. The expression Spreading Resistance derives
Part I Amorphous and Polycrystalline Thin-Film Transistors HYBRID AMORPHOUS AND POLYCRYSTALLINE SILICON DEVICES FOR LARGE-AREA ELECTRONICS P. Mei, J. B. Boyce, D. K. Fork, G. Anderson, J. Ho, J. Lu, Xerox
Chapter 3 Fabrication of CMOS Integrated Circuits Jin-Fu Li Department of Electrical Engineering National Central University Jungli, Taiwan Background Outline The CMOS Process Flow Design Rules Latchup
Defects and Diffusion Goals for the Unit Recognize various imperfections in crystals Point imperfections Impurities Line, surface and bulk imperfections Define various diffusion mechanisms Identify factors
OpenStax-CNX module: m24908 1 Oxidation of Silicon Andrew R. Barron This work is produced by OpenStax-CNX and licensed under the Creative Commons Attribution License 3.0 note: This module was developed
University of Texas Arlington Department of Electrical Engineering Nanotechnology Microelectromechanical Systems Ph.D. Diagnostic Examination Fall 2012 November 17, 2012 Question # 1 2 3 To be filled by
3.155J / 6.152J MICROELECTRONICS PROCESSING TECHNOLOGY TAKE-HOME QUIZ FALL TERM 2003 1) This is an open book, take-home quiz. You are not to consult with other class members or anyone else. You may discuss
Thermal Oxidation and Growth of Insulators (Chapter 3 - Jaeger 3) Key advantage of Si: Oxidation of Si into SiO (glass) Major factor in making Silicon the main semiconductor Grown at high temperature in
Imperfections: Good or Bad? Structural imperfections (defects) Compositional imperfections (impurities) 1 Structural Imperfections A perfect crystal has the lowest internal energy E Above absolute zero